InGaAs/InP quantum well infrared
photodetector integrated on Si substrate by
Mo/Au metal-assisted wafer bonding
MIN-SU PARK, MOHSEN REZAEI, IMAN NIA, ROBERT BROWN, SIMONE
BIANCONI, CHEE LEONG TAN, AND HOOMAN MOHSENI*
Bio-inspired Sensors and Optoelectronics Laboratory (BISOL), EECS, Northwestern University, 2145
Sheridan Rd, Evanston, IL 60208, USA
Abstract: Integration of an InGaAs/InP quantum well infrared photodetector (QWIP) onto a
Si substrate was successfully demonstrated via a metal-assisted wafer bonding (MWB) using
a Mo/Au metal scheme. The Mo/Au/Mo layer, situated between the QWIP structure and the
Si, has shown a well-ordered lamination. It provides a smooth surface with a roughness of
about 0.8 nm, as measured by a scanning electron microscope (SEM) and atomic force
microscopy (AFM). The results on crystalline quality evaluated by Raman spectroscopy and
X-ray diffraction (XRD) imply that the MWB could be achieved without any measurable
material degradation and residual strain. Temperature dependence of dark current revealed
that there is no noticeable change in the dark current properties of the QWIP after bonding on
Si, despite that the quantum wells are only 200 nm away from the bonding interface.
© 2018 Optical Society of America under the terms of the OSA Open Access Publishing Agreement
OCIS codes: (040.5160) Photodetectors; (230.5590) Quantum-well, -wire and -dot devices; (040.6040) Silicon.
References and links
1. B. F. Levine, “Quantum‐well infrared photodetectors,” J. Appl. Phys. 74(8), R1–R81 (1993).
2. A. Rogalski, “Quantum well photoconductors in infrared detector technology,” J. Appl. Phys. 93(8), 4355–4391
3. S. D. Gunapala, S. V. Bandara, J. K. Liu, C. J. Hill, S. B. Rafol, J. M. Mumolo, J. T. Trinh, M. Z. Tidrow, and P.
D. LeVan, “1024 × 1024 pixel mid-wavelength and long-wavelength infrared QWIP focal plane arrays for
imaging applications,” Semicond. Sci. Technol. 20(5), 473–480 (2005).
4. Q. Huang, G. Xu, Y. Yuan, X. Cheng, and L. Luo, “Development of indium bumping technology through
AZ9260 resist electroplating,” J. Micromech. Microeng. 20(5), 055035 (2010).
5. J. Jiang, S. Tsao, T. O’Sullivan, M. Razeghi, and G. J. Brown, “Fabrication of indium bumps for hybrid infrared
focal plane array applications,” Infrared Phys. Technol. 45(2), 143–151 (2004).
6. J. Wu, Q. Jiang, S. Chen, M. Tang, Y. I. Mazur, Y. Maidaniuk, M. Benamara, M. P. Semtsiv, W. T. Masselink,
K. A. Sablon, G. J. Salamo, and H. Liu, “Monolithically Integrated InAs/GaAs Quantum Dot Mid-Infrared
Photodetectors on Silicon Substrates,” ACS Photonics 3(5), 749–753 (2016).
7. S. Chen, M. Tang, Q. Jiang, J. Wu, V. G. Dorogan, M. Benamara, Y. I. Mazur, G. J. Salamo, P. Smowton, A.
Seeds, and H. Liu, “InAs/GaAs Quantum-Dot Superluminescent Light-Emitting Diode Monolithically Grown on
a Si substrate,’,” ACS Photonics 1(7), 638–642 (2014).
8. J. Yua, Y. Wang, J. Q. Lu, and R. J. Gutmann, “Low-temperature silicon wafer bonding based on Ti/Si solid-
state amorphization,” Appl. Phys. Lett. 89(9), 092104 (2006).
9. R. H. Horng, S. H. Huang, D. S. Wuu, and C. Y. Chiu, “AlGaInP/mirror/Si light-emitting diodes with vertical
electrodes by wafer bonding,” Appl. Phys. Lett. 82(23), 4011–4013 (2003).
10. M. S. Park, D. M. Geum, J. H. Kyhm, J. D. Song, S. Kim, and W. J. Choi, “InGaP/GaAs heterojunction
phototransistors transferred to a Si substrate by metal wafer bonding combined with epitaxial lift-off,” Opt.
Express 23(21), 26888–26894 (2015).
11. D. M. Geum, M. S. Park, J. Y. Lim, H. D. Yang, J. D. Song, C. Z. Kim, E. Yoon, S. Kim, and W. J. Choi,
“Ultra-high-throughput Production of III-V/Si Wafer for Electronic and Photonic Applications,” Sci. Rep. 6(1),
12. E. Higurashi, D. Chino, T. Suga, and R. Sawada, “Au–Au Surface-Activated Bonding and Its Application to
Optical Microsensors With 3-D Structure,” IEEE J. Sel. Top. Quantum Electron. 15(5), 1500–1505 (2009).
13. E. Jing, B. Xiong, and Y. Wang, “Low-temperature Au–Si wafer bonding,” J. Micromech. Microeng. 20(9),
Vol. 8, No. 2 | 1 Feb 2018 | OPTICAL MATERIALS EXPRESS 413
Journal © 2018 Received 3 Oct 2017; revised 1 Dec 2017; accepted 4 Dec 2017; published 18 Jan 2018
14. A.G. Bacaa, F. Renb, J.C. Zolper, R.D. Briggsa and S.J. Peartonc, “A survey of ohmic contacts to III-V
compound semiconductors,” Thin Solid Films 308−309, 599−606 (1997).
15. A. K. Baraskar, M. A. Wistey, V. Jain, U. Singisetti, G. Burek, B. J. Thibeault, Y. J. Lee, A. C. Gossard, and M.
J. W. Rodwell, “Ultralow resistance, nonalloyed Ohmic contacts to n-InGaAs,” J. Vac. Sci. Technol. B 27(4),
16. G. Liu, G. J. Zhang, F. Jiang, X. D. Ding, Y. J. Sun, J. Sun, and E. Ma, “Nanostructured high-strength
molybdenum alloys with unprecedented tensile ductility,” Nat. Mater. 12(4), 344–350 (2013).
17. P. Fay, K. Stevens, J. Elliot, and N. Pan, “Performance Dependence of InGaP/InGaAs/GaAs pHEMT’s on Gate
Metallization,” IEEE Electron Device Lett. 20(11), 554–556 (1999).
18. Y. Kitaura, T. Hashimoto, T. Inoue, K. Ishida, N. Uchitomi, and R. Nii, “Long-term reliability of Pt and Mo
diffusion barriers in Ti-Pt-Au and Ti-Mo-Au metallization systems for GaAs digital integrated circuits,” J. Vac.
Sci. Technol. 12(5), 2985–2991 (1994).
19. A. Gupta, D. Paramanik, S. Varma, and C. Jacob, “CVD growth and characterization of 3C-SiC thin films,”
Bull. Mater. Sci. 27(5), 445–451 (2004).
20. M. S. Park, V. Jain, E. H. Lee, S. H. Kim, H. Pettersson, Q. Wang, J. D. Song, and W. J. Choi, “InAs/GaAs p–i–
p quantum dots-in-a-well infrared photodetectors operating beyond 200 K,” Electron. Lett. 50(23), 1731–1733
21. E. Altin, M. Hostut, and Y. Ergun, “Barrier lowering effect and dark current characteristics in asymmetric
GaAs/AlGaAs multi quantum well structure,” Appl. Phys., A Mater. Sci. Process. 105(4), 833–839 (2011).
Compound semiconductor based quantum well infrared photodetectors (QWIPs) have been
showing a tremendous progress for infrared (IR) applications such as high resolution IR
imaging from space, medical diagnosis, monitoring environment, and surveillance [1–3].
Since technology for growth and fabrication of this material system have been developed
continually, large format arrays having a high pixel uniformity and operability can be mass
produced . Such focal plane arrays (FPAs) are typically connected to Si-based readout
integrated circuits (ROICs) through indium bump and flip-chip bonding process, so that the
hybrid integrated chip provides an integrated IR imaging sensor. However, indium bumping
technology has limitation of high-throughput due to the tedious processes, and the fact that it
is a die-level process. Although the indium bumps on the both sides are interconnected by
flip-chip bonding, the unintentionally formed indium oxide on the surface of the bumps
induces to decrease shear strength of the interconnection , and displacement of the indium
bump by thermal cycle between liquid nitrogen and room temperature is incurred .
Furthermore, it is hard to implement the wafer-scale integration, which is the main bottleneck
in mass-production of the non-silicon integrated IR imaging sensors.
In order to circumvent such integration issues, two principal different paths been
considered. One approach is monolithic growth of compound semiconductor on Si platform
(ROICs), using molecular beam epitaxy (MBE) or metalorganic chemical vapor deposition
(MOCVD). They have an advantage of CMOS-compatible fabrication, and hence large
format size and cost effectiveness. Only recently has it become possible to realize the
competitive device performance by achieving a good quality of buffer layers on Si [6, 7].
However, the intrinsic threading dislocation density of the device films, which originated
from the lattice mismatch and thermal expansion coefficient difference from Si, is still an
impediment to their practical use and commercialization. Besides, the high temperature
process to remove the native oxide or contaminants in the growth chamber is virtually
impossible to be applied to fully processed ROICs . On the other hand, metal-assisted
wafer bonding (MWB) has been used. It effectively utilizes an intermediate thin metal to
bond each other wafers. Gold−Gold (Au−Au) bonding has been extensively studied to
implement the integration of compound semiconductor based device on the Si platform by
taking advantage of a low-temperature process that prevents residual stress responsible for
bowing or cracks [8–11]. Moreover, shear strength of Au-Au bonding has been as high as ~20
MPa [12, 13], promising a strong interconnection between the FPA and ROIC for
applications in harsh environments. However, this method suffers from a propensity for deep
spiking, poor controllability, and insufficient thermal stability over 300°C . In order to
avoid the unfavorable diffusion of Au atoms, a good diffusion barrier prior to Au deposition
Vol. 8, No. 2 | 1 Feb 2018 | OPTICAL MATERIALS EXPRESS 414